| Sample code  | Glass transition temperature (degC) | Glass transition temperature (degC) | Crystallization temperature (degC) | Crystallization temperature (degC) | Liquidus temperature (degC) | Liquidus temperature (degC) | Liquidus temperature (degC) | Average bond enthalpy (kJmol-1) |
| Sample code  | Tg1                                 | Tg2                                 | Tc1                                | Tc2                                | Tm1                         | Tm2                         | Tm3                         | Average bond enthalpy (kJmol-1) |
| 20BTe        | 352                                 | -                                   | 447                                | 491                                | 684                         | 689                         | 696                         | 345                             |
| 5Al20BTe     | 366                                 | -                                   | 481                                | 489                                | 673                         | -                           | -                           | 355                             |
| 10Al20BTe    | 379                                 | 440                                 | 524                                | -                                  | 635                         | -                           | -                           | 363                             |
| 5W20BTe      | 358                                 | -                                   | 464                                | 502                                | 603                         | 665                         | -                           | 368                             |
| 5W5Al20BTe   | 373                                 | -                                   | 497                                | -                                  | 639                         | -                           | -                           | 376                             |
| 5W10Al20BTe  | 350                                 | 388                                 | 524                                | 627                                | -                           | -                           | -                           | 381                             |
| 5Nb20BTe     | 369                                 | -                                   | 500                                | 569                                | 658                         | -                           | -                           | 369                             |
| 5Nb5Al20BTe  | 383                                 | -                                   | 624                                | -                                  | 688                         | -                           | -                           | 374                             |
| 5Nb10Al20BTe | 326                                 | 401                                 | 635                                | -                                  | -                           | -                           | -                           | 381                             |
| 5Pb20BTe     | 340                                 | -                                   | 418                                | 521                                | 681                         | -                           | -                           | 338                             |
| 5Pb5Al20BTe  | 356                                 | -                                   | 455                                | -                                  | 647                         | -                           | -                           | 345                             |
| 5Pb10Al20BTe | 323                                 | 386                                 | 528                                | 617                                | -                           | -                           | -                           | 355                             |

Caption: Glass transition (midpoint value), crystallization (peak point) and liquidus (peak point) temperatures of glasses. Maximum uncertainty in the temperatures values is +-1degC.

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "352", "type": "Other"}
{"value": "447", "type": "Other"}
{"value": "491", "type": "Other"}
{"value": "684", "type": "Other"}
{"value": "689", "type": "Other"}
{"value": "696", "type": "Other"}
{"value": "345", "type": "Other"}
{"value": "366", "type": "Other"}
{"value": "481", "type": "Other"}
{"value": "489", "type": "Other"}
{"value": "673", "type": "Other"}
{"value": "355", "type": "Other"}
{"value": "379", "type": "Other"}
{"value": "440", "type": "Other"}
{"value": "524", "type": "Other"}
{"value": "635", "type": "Other"}
{"value": "363", "type": "Other"}
{"value": "358", "type": "Other"}
{"value": "464", "type": "Other"}
{"value": "502", "type": "Other"}
{"value": "603", "type": "Other"}
{"value": "665", "type": "Other"}
{"value": "368", "type": "Other"}
{"value": "373", "type": "Other"}
{"value": "497", "type": "Other"}
{"value": "639", "type": "Other"}
{"value": "376", "type": "Other"}
{"value": "350", "type": "Other"}
{"value": "388", "type": "Other"}
{"value": "524", "type": "Other"}
{"value": "627", "type": "Other"}
{"value": "381", "type": "Other"}
{"value": "369", "type": "Other"}
{"value": "500", "type": "Other"}
{"value": "569", "type": "Other"}
{"value": "658", "type": "Other"}
{"value": "369", "type": "Other"}
{"value": "383", "type": "Other"}
{"value": "624", "type": "Other"}
{"value": "688", "type": "Other"}
{"value": "374", "type": "Other"}
{"value": "326", "type": "Other"}
{"value": "401", "type": "Other"}
{"value": "635", "type": "Other"}
{"value": "381", "type": "Other"}
{"value": "340", "type": "Other"}
{"value": "418", "type": "Other"}
{"value": "521", "type": "Other"}
{"value": "681", "type": "Other"}
{"value": "338", "type": "Other"}
{"value": "356", "type": "Other"}
{"value": "455", "type": "Other"}
{"value": "647", "type": "Other"}
{"value": "345", "type": "Other"}
{"value": "323", "type": "Other"}
{"value": "386", "type": "Other"}
{"value": "528", "type": "Other"}
{"value": "617", "type": "Other"}
{"value": "355", "type": "Other"}